Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules


 Verity Singleton
 1 years ago
 Views:
Transcription
1 141 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene (b Poly(vinyl alcohol
2 142 Molecular Weight 14.2 Repeat unit weights for several polymers are asked for in this problem. (a For polytetrafluoroethylene, each repeat unit consists of two carbons and four fluorines (Table If A C and A F represent the atomic weights of carbon and fluorine, respectively, then m 2(A C + 4(A F (2(12.01 g/mol + (4(19.00 g/mol g/mol (b For poly(methyl methacrylate, from Table 14.3, each repeat unit has five carbons, eight hydrogens, and two oxygens. Thus, m 5(A C + 8(A H + 2(A O (5(12.01 g/mol + (8(1.008 g/mol + (2(16.00 g/mol g/mol (c For nylon 6,6, from Table 14.3, each repeat unit has twelve carbons, twentytwo hydrogens, two nitrogens, and two oxygens. Thus, m 12(A C + 22(A H + 2(A N + 2(A O (12(12.01 g/mol + (22(1.008 g/mol + (2(14.01 g/mol + (2(16.00 g/mol g/mol (d For poly(ethylene terephthalate, from Table 14.3, each repeat unit has ten carbons, eight hydrogens, and four oxygens. Thus, m 10(A C + 8(A H + 4(A O (10(12.01 g/mol + (8(1.008 g/mol + (4(16.00 g/mol g/mol
3 We are asked to compute the degree of polymerization for polystyrene, given that the numberaverage molecular weight is 500,000 g/mol. The repeat unit molecular weight of polystyrene is just m 8(A C + 8(A H (8(12.01 g/mol + (8(1.008 g/mol g/mol Now it is possible to compute the degree of polymerization using Equation 14.6 as DP M n m 500,000 g/mol g/mol 4800
4 (a The repeat unit molecular weight of polypropylene is called for in this portion of the problem. For polypropylene, from Table 14.3, each repeat unit has three carbons and six hydrogens. Thus, m 3(A C + 6(A H (3(12.01 g/mol + (6(1.008 g/mol g/mol (b We are now asked to compute the numberaverage molecular weight. Since the degree of polymerization is 15,000, using Equation 14.6 M n (DPm (15,000(42.08 g/mol 631,000 g/mol
5 (a From the tabulated data, we are asked to compute M n, the numberaverage molecular weight. This is carried out below. Molecular wt Range Mean M i x i x i M i 10,00020,000 15, ,00030,000 25, ,00040,000 35, ,00050,000 45, ,250 50,00060,000 55, ,100 60,00070,000 65, ,00080,000 75, ,00090,000 85, M n x i M i 49, 800 g/mol (b From the tabulated data, we are asked to compute M w, the weightaverage molecular weight. Molecular wt. Range Mean M i w i w i M i 10,00020,000 15, ,00030,000 25, ,00040,000 35, ,00050,000 45, ,350 50,00060,000 55, ,200 60,00070,000 65, ,700 70,00080,000 75, ,00090,000 85, M w w i M i 55,200 g/mol (c Now we are asked to compute the degree of polymerization, which is possible using Equation For polytetrafluoroethylene, the repeat unit molecular weight is just
6 146 m 2(A C + 4(A F (2(12.01 g/mol + (4(19.00 g/mol g/mol And DP M n m 49,800 g/mol g/mol 498
7 (a From the tabulated data, we are asked to compute M n, the numberaverage molecular weight. This is carried out below. Molecular wt. Range Mean M i x i x i M i 8,00020,000 14, ,00032,000 26, ,00044,000 38, ,00056,000 50, ,000 56,00068,000 62, ,160 68,00080,000 74, ,00092,000 86, M n x i M i 47, 720 g/mol (b From the tabulated data, we are asked to compute M w, the weightaverage molecular weight. This determination is performed as follows: Molecular wt. Range Mean M i w i w i M i 8,00020,000 14, ,00032,000 26, ,00044,000 38, ,00056,000 50, ,500 56,00068,000 62, ,260 68,00080,000 74, ,840 80,00092,000 86, M w w i M i 53,720 g/mol (c We are now asked if the degree of polymerization is 477, which of the polymers in Table 14.3 is this material? It is necessary to compute m in Equation 14.6 as m M n DP 47,720 g/mol g/mol
8 148 The repeat unit molecular weights of the polymers listed in Table 14.3 are as follows: Polyethylene g/mol Poly(vinyl chloride g/mol Polytetrafluoroethylene g/mol Polypropylene g/mol Polystyrene g/mol Poly(methyl methacrylate g/mol Phenolformaldehyde g/mol Nylon 6, g/mol PET g/mol Polycarbonate g/mol Therefore, polytetrafluoroethylene is the material since its repeat unit molecular weight is closest to that calculated above.
9 This problem asks if it is possible to have a poly(vinyl chloride homopolymer with the given molecular weight data and a degree of polymerization of The appropriate data are given below along with a computation of the numberaverage molecular weight. Molecular wt. Range Mean M i x i x i M i 8,00020,000 14, ,00032,000 26, ,00044,000 38, ,00056,000 50, ,000 56,00068,000 62, ,160 68,00080,000 74, ,00092,000 86, M w x i M i 47,720 g/mol For PVC, from Table 14.3, each repeat unit has two carbons, three hydrogens, and one chlorine. Thus, m 2(A C + 3(A H + (A Cl (2(12.01 g/mol + (3(1.008 g/mol + (35.45 g/mol g/mol Now, we will compute the degree of polymerization using Equation 14.6 as DP M n m 47,720 g/mol g/mol 764 Thus, such a homopolymer is not possible since the calculated degree of polymerization is 764 not 1120.
10 (a For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added for 8% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100 possible sidebonding sites. Ninetytwo are occupied by hydrogen and eight are occupied by Cl. Thus, the mass of these 50 carbon atoms, m C, is just m C 50(A C (50(12.01 g/mol g Likewise, for hydrogen and chlorine, m H 92(A H (92(1.008 g/mol g m Cl 8(A Cl (8(35.45 g/mol g Thus, the concentration of chlorine, C Cl, is determined using a modified form of Equation 4.3 as C Cl m Cl m C + m H + m Cl x g g g g x wt% (b Chlorinated polyethylene differs from poly(vinyl chloride, in that, for PVC, (1 25% of the sidebonding sites are substituted with Cl, and (2 the substitution is probably much less random.
11 1411 Molecular Shape 14.9 This problem first of all asks for us to calculate, using Equation 14.11, the average total chain length, L, for a linear polyethylene polymer having a numberaverage molecular weight of 300,000 g/mol. It is necessary to calculate the numberaverage degree of polymerization, DP, using Equation For polyethylene, from Table 14.3, each repeat unit has two carbons and four hydrogens. Thus, m 2(A C + 4(A H (2(12.01 g/mol + (4(1.008 g/mol g/mol and DP M n m 300,000 g/mol g/mol 10,695 which is the number of repeat units along an average chain. Since there are two carbon atoms per repeat unit, there are two C C chain bonds per repeat unit, which means that the total number of chain bonds in the molecule, N, is just (2(10,695 21,390 bonds. Furthermore, assume that for single carboncarbon bonds, d nm and θ 109 (Section 14.4; therefore, from Equation θ L Nd sin 2 (21,390(0.154 nm sin nm 2 It is now possible to calculate the average chain endtoend distance, r, using Equation as r d N (0.154 nm 21, nm
12 (a This portion of the problem asks for us to calculate the numberaverage molecular weight for a linear polytetrafluoroethylene for which L in Equation is 2000 nm. It is first necessary to compute the value of N using this equation, where, for the C C chain bond, d nm, and θ 109. Thus N L d sin θ nm (0.154 nm sin ,900 Since there are two C C bonds per PTFE repeat unit, there is an average of N/2 or 15,900/ repeat units per chain, which is also the degree of polymerization, DP. In order to compute the value of M n using Equation 14.6, we must first determine m for PTFE. Each PTFE repeat unit consists of two carbon and four fluorine atoms, thus m 2(A C + 4(A F (2(12.01 g/mol + (4(19.00 g/mol g/mol Therefore M n (DPm (7950( g/mol 795,000 g/mol (b Next, we are to determine the numberaverage molecular weight for r 15 nm. Solving for N from Equation leads to N r2 d 2 (15 nm 2 (0.154 nm which is the total number of bonds per average molecule. Since there are two C C bonds per repeat unit, then DP N/2 9490/ Now, from Equation 14.6 M n (DPm (4745( g/mol 474,600 g/mol
13 1413 Molecular Configurations We are asked to sketch portions of a linear polypropylene molecule for different configurations (using twodimensional schematic sketches. (a Syndiotactic polypropylene (b Atactic polypropylene (c Isotactic polypropylene
14 This problem asks for us to sketch cis and trans structures for butadiene and chloroprene. (a The structure for cis polybutadiene (Table 14.5 is The structure of trans butadiene is (b The structure of cis chloroprene (Table 14.5 is The structure of trans chloroprene is
15 1415 Thermoplastic and Thermosetting Polymers This question asks for comparisons of thermoplastic and thermosetting polymers. (a Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting polymers, harden upon heating, while further heating will not lead to softening. (b Thermoplastic polymers have linear and branched structures, while for thermosetting polymers, the structures will normally be network or crosslinked.
16 (a It is not possible to grind up and reuse phenolformaldehyde because it is a network thermoset polymer and, therefore, is not amenable to remolding. (b Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will soften when reheated, and, thus, may be remolded.
17 1417 Copolymers This problem asks for sketches of the repeat unit structures for several alternating copolymers. (a For poly(ethylenepropylene (b For poly(butadienestyrene (c For poly(isobutyleneisoprene
18 For a poly(acrylonitrilebutadiene alternating copolymer with a numberaverage molecular weight of 1,000,000 g/mol, we are asked to determine the average number of acrylonitrile and butadiene repeat units per molecule. Since it is an alternating copolymer, the number of both types of repeat units will be the same. Therefore, consider them as a single repeat unit, and determine the numberaverage degree of polymerization. For the acrylonitrile repeat unit, there are three carbon atoms, three hydrogen atoms, and one nitrogen atom, while the butadiene repeat consists of four carbon atoms and six hydrogen atoms. Therefore, the acrylonitrilebutadiene combined repeat unit weight is just m 7(A C + 9(A H + 1(A N (7(12.01 g/mol + (9(1.008 g/mol + (14.01 g/mol g/mol From Equation 14.6, the degree of polymerization is just DP M n m 1,000,000 g/mol g/mol 9333 Thus, there is an average of 9333 of both repeat unit types per molecule.
19 This problem asks for us to calculate the numberaverage molecular weight of a random poly(isobutyleneisoprene copolymer. For the isobutylene repeat unit there are four carbon and eight hydrogen atoms. Thus, its repeat unit molecular weight is m Ib 4(A C + 8(A H (4(12.01 g/mol + (8(1.008 g/mol g/mol The isoprene repeat unit is composed of five carbon and eight hydrogen atoms. Thus, its repeat unit molecular weight is m Ip 5(A C + 8(A H (5(12.01 g/mol + (8(1.008 g/mol g/mol From Equation 14.7, the average repeat unit molecular weight is just m f Ib m Ib + f Ip m Ip (0.25(56.10 g/mol + (0.75(68.11 g/mol g/mol Since DP 1500 (as stated in the problem, M n may be computed using Equation 14.6 as M n m (DP (65.11 g/mol( ,700 g/mol
20 For an alternating copolymer that has a numberaverage molecular weight of 100,000 g/mol and a degree of polymerization of 2210, we are to determine one of the repeat unit types if the other type is ethylene. It is first necessary to calculate m using Equation 14.6 as m M n DP 100,000 g/mol g/mol Since this is an alternating copolymer we know that chain fraction of each repeat unit type is 0.5; that is f e f x 0.5, f e and f x being, respectively, the chain fractions of the ethylene and unknown repeat units. Also, the repeat unit molecular weight for ethylene is m s 2(A C + 4(A H 2(12.01 g/mol + 4(1.008 g/mol g/mol Now, using Equation 14.7, it is possible to calculate the repeat unit weight of the unknown repeat unit type, m x. Thus m x m f e m e f x g/mol  (0.5(28.05 g/mol g/mol Finally, it is necessary to calculate the repeat unit molecular weights for each of the possible other repeat unit types. These are calculated below: m styrene 8(A C + 8(A H 8(12.01 g/mol + 8(1.008 g/mol g/mol m propylene 3(A C + 6(A H 3(12.01 g/mol + 6(1.008 g/mol g/mol m TFE 2(A C + 4(A F 2(12.01 g/mol + 4(19.00 g/mol g/mol m VC 2(A C + 3(A H + (A Cl 2(12.01 g/mol + 3(1.008 g/mol g/mol g/mol Therefore, vinyl chloride is the other repeat unit type since its m value is almost the same as the calculated m x.
21 (a This portion of the problem asks us to determine the ratio of butadiene to acrylonitrile repeat units in a copolymer having a weightaverage molecular weight of 250,000 g/mol and a degree of polymerization of It first becomes necessary to calculate the average repeat unit molecular weight of the copolymer, m, using Equation 14.6 as m M n DP 250,000 g/mol g/mol If we designate f b as the chain fraction of butadiene repeat units, since the copolymer consists of only two repeat unit types, the chain fraction of acrylontrile repeat units f a is just 1 f b. Now, Equation 14.7 for this copolymer may be written in the form m f b m b + f a m a f b m b + (1 f b m a in which m b and m a are the repeat unit molecular weights for butadiene and acrylontrile, respectively. These values are calculated as follows: m b 4(A C + 6(A H 4(12.01 g/mol + 6(1.008 g/mol g/mol m a 3(A C + 3(A H + (A N 3(12.01 g/mol + 3(1.008 g/mol + (14.01 g/mol g/mol. Solving for f b in the above expression yields f b m m a m b m a g/mol g/mol g/mol g/mol 0.80 Furthermore, f a 1 f b ; or the ratio is just f b f a (b Of the possible copolymers, the only one for which there is a restriction on the ratio of repeat unit types is alternating; the ratio must be 1:1. Therefore, on the basis of the result in part (a, the possibilities for this copolymer are random, graft, and block.
22 For a copolymer consisting of 35 wt% ethylene and 65 wt% propylene, we are asked to determine the fraction of both repeat unit types. In 100 g of this material, there are 35 g of ethylene and 65 g of propylene. The ethylene (C 2 H 4 molecular weight is m(ethylene 2(A C + 4(A H (2(12.01 g/mol + (4(1.008 g/mol g/mol The propylene (C 3 H 6 molecular weight is m(propylene 3(A C + 6(A H (3(12.01 g/mol + (6(1.008 g/mol g/mol Therefore, in 100 g of this material, there are 35 g 1.25 mol of ethylene g /mol and 65 g 1.54 mol of propylene g /mol Thus, the fraction of the ethylene repeat unit, f(ethylene, is just f (ethylene 1.25 mol 1.25 mol mol 0.45 Likewise, f (propylene 1.54 mol 1.25 mol mol 0.55
23 For a random poly(styrenebutadiene copolymer in which M n 350,000 g/mol and DP 5000, we are asked to compute the fractions of styrene and butadiene repeat units. From Table 14.5, the styrene repeat unit has eight carbon and eight hydrogen atoms. Thus, m st (8(12.01 g/mol + (8(1.008 g/mol g/mol Also, from Table 14.5, the butadiene repeat unit has four carbon and six hydrogen atoms, and m bu (4(12.01 g/mol + (6(1.008 g/mol g/mol From Equation 14.7 m f st m st + f bu m bu Now, let x f st, such that m x + (54.09(1 x since f st + f bu 1. Also, from Equation 14.6 Or DP M n m ,000 g /mol [ x (1 x] g /mol Solving for x leads to x f st f(styrene Also, f(butadiene 1 x
24 1424 Polymer Crystallinity The tendency of a polymer to crystallize decreases with increasing molecular weight because as the chains become longer it is more difficult for all regions along adjacent chains to align so as to produce the ordered atomic array.
25 For each of four pairs of polymers, we are asked to (1 state whether it is possible to decide which is more likely to crystallize; (2 if so, which is more likely and why; and (3 it is not possible to decide then why. (a No, it is not possible to decide for these two polymers. On the basis of tacticity, the isotactic PP is more likely to crystallize than the atactic PVC. On the other hand, with regard to sidegroup bulkiness, the PVC is more likely to crystallize. (b Yes, it is possible to decide for these two copolymers. The linear and syndiotactic polypropylene is more likely to crystallize than crosslinked cisisoprene since linear polymers are more likely to crystallize than crosslinked ones. (c Yes, it is possible to decide for these two polymers. The linear and isotactic polystyrene is more likely to crystallize than network phenolformaldehyde; network polymers rarely crystallize, whereas isotactic ones crystallize relatively easily. (d Yes, it is possible to decide for these two copolymers. The block poly(acrylonitrileisoprene copolymer is more likely to crystallize than the graft poly(chloropreneisobutylene copolymer. Block copolymers crystallize more easily than graft ones.
26 For this problem we are given the density of nylon 6,6 (1.213 g/cm 3, an expression for the volume of its unit cell, and the lattice parameters, and are asked to determine the number of repeat units per unit cell. This computation necessitates the use of Equation 3.5, in which we solve for n. Before this can be carried out we must first calculate V C, the unit cell volume, and A the repeat unit molecular weight. For V C V C abc 1 cos 2 α cos 2 β cos 2 γ + 2 cosα cosβ cos γ (0.497(0.547( (0.664(0.232( nm x cm 3 The repeat unit for nylon 6,6 is shown in Table 14.3, from which the value of A may be determined as follows: A 12(A C + 22(A H + 2(A O + 2(A N 12(12.01 g/mol + 22(1.008 g/mol + 2(16.00 g/mol + 2(14.01 g/mol g/mol Finally, solving for n from Equation 3.5 leads to n ρv C N A A (1.213 g/cm3 (3.098 x cm 3 /unit cell(6.023 x repeat units/mol g/mol 1 repeat unit/unit cell
27 (a We are asked to compute the densities of totally crystalline and totally amorphous poly(ethylene terephthalate (ρ c and ρ a from Equation From Equation 14.8 let C % crystallinity, such that 100 C ρ c (ρ s ρ a ρ s (ρ c ρ a Rearrangement of this expression leads to ρ c (C ρ s ρ s + ρ c ρ a Cρ s ρ a 0 in which ρ c and ρ a are the variables for which solutions are to be found. Since two values of ρ s and C are specified in the problem statement, two equations may be constructed as follows: ρ c (C 1 ρ s1 ρ s1 + ρ c ρ a C 1 ρ s1 ρ a 0 ρ c (C 2 ρ s2 ρ s2 + ρ c ρ a C 2 ρ s2 ρ a 0 In which ρ s g/cm 3, ρ s g/cm 3, C , and C Solving the above two equations for ρ a and ρ c leads to ρ a ρ s1 ρ s2 (C 1 C 2 C 1 ρ s1 C 2 ρ s2 (1.408 g/cm 3 (1.343 g/cm 3 ( (0.743(1.408 g/cm 3 (0.312(1.343 g/cm g/cm3 And ρ c ρ s1 ρ s2 (C 2 C 1 ρ s2 (C 2 1 ρ s1 (C 1 1 (1.408 g/cm 3 (1.343 g/cm 3 ( (1.343 g/cm 3 ( (1.408 g/cm 3 ( g/cm3 (b Now we are to determine the % crystallinity for ρ s g/cm 3. Again, using Equation 14.8
28 1428 % crystallinity ρ c (ρ s ρ a ρ s (ρ c ρ a 100 (1.450 g/cm3 (1.382 g/cm g/cm 3 (1.382 g/cm 3 (1.450 g/cm g/cm %
29 (a We are asked to compute the densities of totally crystalline and totally amorphous polypropylene (ρ c and ρ a from Equation From Equation 14.8 let C % crystallinity, such that 100 C ρ c (ρ s ρ a ρ s (ρ c ρ a Rearrangement of this expression leads to ρ c (C ρ s ρ s + ρ c ρ a C ρ s ρ a 0 in which ρ c and ρ a are the variables for which solutions are to be found. Since two values of ρ s and C are specified in the problem, two equations may be constructed as follows: ρ c (C 1 ρ s1 ρ s1 + ρ c ρ a C 1 ρ s1 ρ a 0 ρ c (C 2 ρ s2 ρ s2 + ρ c ρ a C 2 ρ s2 ρ a 0 In which ρ s g/cm 3, ρ s g/cm 3, C , and C Solving the above two equations for ρ a and ρ c leads to ρ a ρ s1 ρ s2 (C 1 C 2 C 1 ρ s1 C 2 ρ s2 (0.904 g /cm3 (0.895 g /cm 3 ( (0.628(0.904 g /cm 3 (0.544(0.895 g /cm g/cm3 And ρ c ρ s1 ρ s2 (C 2 C 1 ρ s2 (C 2 1 ρ s1 (C 1 1 (0.904 g /cm 3 (0.895 g /cm 3 ( (0.895 g /cm 3 ( (0.904 g /cm g/cm3 ( (b Now we are asked to determine the density of a specimen having 74.6% crystallinity. Solving for ρ s from Equation 14.8 and substitution for ρ a and ρ c which were computed in part (a yields
30 1430 ρ s ρ c ρ a C (ρ c ρ a ρ c (0.946 g /cm 3 (0.841 g /cm 3 (0.746(0.946 g /cm g /cm g /cm g/cm 3
31 1431 Diffusion in Polymeric Materials This is a permeability problem in which we are asked to compute the diffusion flux of oxygen through a 15mm thick sheet of low density polyethylene. In order to solve this problem it is necessary to employ Equation The permeability coefficient of O 2 through LDPE is given in Table 14.6 as 2.2 x (cm 3 STP cm/cm 2 spa. Thus, from Equation 14.9 J P M P x P M P 2 P 1 x and taking P kpa (150,000 Pa and P kpa (2,000,000 Pa we get 2.2 x (cm 3 STP(cm 2,000,000 Pa  150, 000 Pa cm 2 spa 1.5 cm 2.7 x 106 (cm 3 STP cm 2 s
32 This problem asks us to compute the permeability coefficient for carbon dioxide through high density polyethylene at 325 K given a steadystate permeability situation. It is necessary for us to Equation 14.9 in order to solve this problem. Rearranging this expression and solving for the permeability coefficient gives P M J x P J x P 2 P 1 Taking P kpa (2,500,000 Pa and P kpa (4,000,000 Pa, the permeability coefficient of CO 2 through HDPE is equal to 2.2 x 108 (cm 3 STP cm 2 (5 cm s P M (4,000,000 Pa  2,500,000 Pa 0.73 x (cm 3 STP(cm cm 2 spa
33 This problem asks that we compute the diffusion flux at 350 K for water in polystyrene. It is first necessary to compute the value of the permeability coefficient at 350 K. The temperature dependence of P M is given in the problem statement, as follows: P M P M0 exp Q p RT And, incorporating values provided for the constants P M0 and Q p, we get P M 9.0 x 105 (cm 3 STP(cm cm 2 spa exp 42,300 J/mol (8.314 J/mol K(350 K 4.4 x (cm 3 STP(cm cm 2 spa And, using Equation 14.9, the diffusion flux is equal to J P M P x P M P 2 P 1 x 4.4 x (cm 3 STP(cm cm 2 spa 20,000 Pa 1,000 Pa 3.0 cm 2.8 x 107 (cm 3 STP cm 2 s
Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules
141 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene
More informationM n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol
14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit
More informationHW 10. = 3.3 GPa (483,000 psi)
HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;
More information15.32 Of those polymers listed in Table 15.2, which polymer(s) would be best suited for use as ice cube trays? Why?
15.31 Name the following polymer(s) that would be suitable for the fabrication of cups to contain hot coffee: polyethylene, polypropylene, poly(vinyl chloride), PET polyester, and polycarbonate. Why? This
More informationPolymers: Introduction
Chapter Outline: Polymer Structures Hydrocarbon and Polymer Molecules Chemistry of Polymer Molecules Molecular Weight and Shape Molecular Structure and Configurations Copolymers Polymer Crystals Optional
More informationEngr Materials Science and Engineering TEST 4  Sample Solution
Engr 70  Materials Science and Engineering TEST 4  Sample Solution Part : Solve each of the following problems completely. 1. In this problem we are asked to show that the minimum cationtoanion radius
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationLecture 4.1: Thermoplastics and Thermosets
Lecture 4.1: Thermoplastics and Thermosets The word plastic comes from the Greek word Plastikos, meaning able to be shaped and molded. Plastics can be broadly classified into two major groups on the basis
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationEffect of Sterilization Techniques on Polymers
Effect of Sterilization Techniques on Polymers Contents of Presentation Introduction to Polymers Properties and Stability of Polymers Affect of Ionising Radiation and Ethylene Oxide on Polymers The need
More informationCHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS
191 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of
More informationElements of Addition Polymerization. Branching and Tacticity. The Effect of Crystallinity on Properties
Topics to be Covered Elements of Addition Polymerization Branching and Tacticity The Effect of Crystallinity on Properties Chapters 1 & 2 in CD (Polymer Science and Engineering) What Are Polyolefins? The
More informationPolymer Chemistry. 3.1 What is a Polymer?
3 asic Polymer hemistry Polymer chemistry is a very complex subject. The basic information presented here is sufficient for the reader to gain a good understanding of polymers which forms the base for
More informationTechnical Reference on Hydrogen Compatibility of Materials
Technical Reference on Hydrogen Compatibility of Materials Nonmetals: (code 8100) Prepared by: C. San Marchi, Sandia National Laboratories, Livermore CA Editors C. San Marchi B.P. Somerday Sandia National
More informationSORTING PLASTICS FOR RECYCLING INTRODUCTION
SORTING PLASTICS FOR RECYCLING INTRODUCTION Description Students use the difference in densities of polymers and flame tests as a basis for the development of a scheme to separate plastics. Goals for This
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationPolymer contains repeating units. A polymer is a macromolecule...but a macromolecule may not be a polymer
Polymer contains repeating units Macromolecules contain no repeating units, examples are DNA, proteins, etc A polymer is a macromolecule...but a macromolecule may not be a polymer Many + Parts The repeating
More informationResistance of Plastics to Gamma Irradiation
Elastomers 1 MATERIAL TOLERANCE LEVEL (kgy) COMMENTS Butyl 50 Sheds particulate after irradiation. Ethylene Propylene 100 200 Crosslinks, yellows slightly. Diene Monomer (EPDM) Fluoro Elastomer 50 Avoid
More informationAlcohols. Characterized by OH group Name: add ol. to name of hydrocarbon. Methanol. Butanol. Sterno. Alcohols burn in air. A mixture of ethanol +
1 2 3 Functional Groups Alcohols Structures of Alcohols haracterized by group Name: add ol to name of hydrocarbon 3 5 : how many structural isomers? See DRM Screens 11.5 & 11.6 Methanol Butanol 1propanol
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationOUT SIDE BACK COVER OUT SIDE FRONT COVER
OUT SIDE BACK COVER OUT SIDE FRONT COVER CONTENT IRPC OVERVIEW PETROCHEMICAL BUSINESS POLYOLEFINS PRODUCTS 8 HDPE 9 HDPE PIPE COMPOUND 10 PP HOMOPOLYMER 11 PP BLOCK COPOLYMER 12 PP RANDOM COPOLYMER 13
More informationF321 MOLES. Example If 1 atom has a mass of 1.241 x 1023 g 1 mole of atoms will have a mass of 1.241 x 1023 g x 6.02 x 10 23 = 7.
Moles 1 MOLES The mole the standard unit of amount of a substance (mol) the number of particles in a mole is known as Avogadro s constant (N A ) Avogadro s constant has a value of 6.02 x 10 23 mol 1.
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationPLASTICS AND ELASTOMERS
THE EFFECT OF STERILIZATION ON PLASTICS AND ELASTOMERS Third Edition Laurence McKeen ELSEVIER Amsterdam Boston Heidelberg London New York Oxford Paris San Diego San Francisco Singapore Sydney Tokyo William
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationPacking materials. Vagn Handlos, Senior scientist, Capital Region Pharmacy, Copenhagen Director of Education, Science and Research EAHP.
Packing materials Vagn Handlos, Senior scientist, Capital Region Pharmacy, Copenhagen Director of Education, Science and Research EAHP. but: Disclosure for Vagn Handlos Nothing to disclose! Assigned professor,
More informationMATERIAL COMPATIBILITY
Asahi Glass Co., Ltd. ASAHIKLIN AK225AES INTRODUCTION ASAHIKLIN AK225AES was developed as a defluxing agent. AK225AES is an azeotropelike mixture of AK225, ethanol and stabilizer and is suitable for
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationSection 5 Plastic & Thermoplastic Elastomer Materials
Section 5 Plastic & Thermoplastic Elastomer Materials High Performance Plastics................... Superior Performance...................... Thermoset Plastics vs Thermoplastics.......... Temperature
More informationMeasurement of Tg by DSC
application note Measurement of Tg by DSC W.J. Sichina What is Tg? Tg is the accepted abbreviation for the glass transition temperature. All amorphous (noncrystalline or semicrystalline) materials will
More informationFriction and Wear of Polymers and Composites. Why do we use polymeric bearings?
Friction and Wear of Polymers and Composites Why do we use polymeric bearings? Low friction No need to lubricate Biocompatible Ease of manufacturing Low noise Low cost 1 Applications of Polymeric Bearings
More informationSYNTHETIC MACROMOLECULAR SUBSTANCES
History: 1. Materials made by chemical modification of natural polymers: EBONITE (Ch. Goodyear, 1851) = hard rubber made by... (treatment with sulphur) of natural rubber, originally electric insulator
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS
CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Atomic structure relates to the number of
More informationCHEMICAL ENGINEERING AND CHEMICAL PROCESS TECHNOLOGY Petrochemicals C. R. Deddis
PETROCHEMICALS C. R. Deddis BP Exploration Operating Company Ltd., UK Keywords: Petrochemicals, hydrocarbons, natural gas, cracking, olefins, aromatics, polymers, fibers. Contents 1. Introduction 2. Petrochemicals
More informationStrength and Stiffness
Strength and Stiffness Stress = load/area is applied to a material by loading it Strain = deformation/length a change of shape (dimensions and twist angles) is its response Stiffness = stress/strain is
More information20.2 Chemical Equations
All of the chemical changes you observed in the last Investigation were the result of chemical reactions. A chemical reaction involves a rearrangement of atoms in one or more reactants to form one or more
More informationChapter 15: Processing of Polymers
Chapter 15: Characteristics, Applications & Processing of Polymers ISSUES TO ADDRESS... What are the tensile properties of polymers and how are they affected by basic microstructural features? Hardening,
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationCHAPTER 12 GASES AND THEIR BEHAVIOR
Chapter 12 Gases and Their Behavior Page 1 CHAPTER 12 GASES AND THEIR BEHAVIOR 121. Which of the following represents the largest gas pressure? (a) 1.0 atm (b) 1.0 mm Hg (c) 1.0 Pa (d) 1.0 KPa 122. Nitrogen
More informationCHEM 121 Chapter 13. Name: Date:
CHEM 121 Chapter 13. Name: Date: 1. The common feature found in all unsaturated hydrocarbons is A) one or more carboncarbon double bonds. B) one or more carboncarbon triple bonds. C) one or more carboncarbon
More informationMULTIPLE CHOICE 1. What are standard temperature and pressure conditions for gases?
Gas Laws MULTIPLE CHOICE 1. What are standard temperature and pressure conditions for gases? a. 0 C and 0 torr b. 0 K and 760 torr c. 273 C and 1 atm d. 0 C and 760 torr e. 0 C and 1 torr 2. If the volume
More informationBack to Basics Fundamentals of Polymer Analysis
Back to Basics Fundamentals of Polymer Analysis Using Infrared & Raman Spectroscopy Molecular Spectroscopy in the Polymer Manufacturing Process Process NIR NIR Production Receiving Shipping QC R&D Routine
More information1. The percent by mass of nitrogen in Mg(CN) 2 is equal to 1) 3)
1. The percent by mass of nitrogen in Mg(CN) 2 is equal to 2. A compound consists of 40.% sulfur and 60.% oxygen by mass. What is the empirical formula of this compound? 1) SO 2) SO 2 3) SO 3 4) SO 4 3.
More informationProblem Set 2 Solutions
Chemistry 360 Dr. Jean M. Standard roblem Set Solutions 1. The atmospheric surface pressure on Venus is 90 bar. The atmosphere near the surface is composed of 96% carbon dioxide and 4% other gases. Given
More information(a) Given that the spacing between polymer chains in PP and PVC is similar, the beads that sink are made of which polymer? Explain.
A student places a mixture of plastic beads consisting of polypropylene (PP) and polyvinyl chloride (PVC) in a 1.0 L beaker containing distilled water. After stirring the contents of the beaker vigorously,
More informationCHEMISTRY. (i) It failed to explain how atoms of different elements differ from each other.
CHEMISTRY MOLE CONCEPT DALTON S ATOMIC THEORY By observing the laws of chemical combination, John Dalton proposed an atomic theory of matter. The main points of Dalton s atomic theory are as follows: (i)
More informationPage 1. 6. Which hydrocarbon is a member of the alkane series? (1) 1. Which is the structural formula of methane? (1) (2) (2) (3) (3) (4) (4)
1. Which is the structural formula of methane? 6. Which hydrocarbon is a member of the alkane series? 7. How many carbon atoms are contained in an ethyl group? 1 3 2 4 2. In the alkane series, each molecule
More informationStress Strain Behavior (I) Stress Strain Behavior (II) Stress Strain Behavior (III)
Chapter Outline: Characteristics, Applications, and Processing of Polymers Mechanical properties StressStrain Behavior Deformation of Semicrystalline Polymers Crystallization, Melting, Glass Transition
More informationAS1 MOLES. oxygen molecules have the formula O 2 the relative mass will be 2 x 16 = 32 so the molar mass will be 32g mol 1
Moles 1 MOLES The mole the standard unit of amount of a substance the number of particles in a mole is known as Avogadro s constant (L) Avogadro s constant has a value of 6.023 x 10 23 mol 1. Example
More informationPhysics Courseware Physics I Ideal Gases
Physics Courseware Physics I Ideal Gases Problem 1. How much mass of helium is contained in a 0.0 L cylinder at a pressure of.0 atm and a temperature of.0 C? [The atomic mass of helium is 4 amu] PV (
More information14:635:407:02 Homework III Solutions
14:635:407:02 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationPolypropylene Alternatives for Medium Voltage Cable Jackets
Polypropylene Alternatives for Medium Voltage Cable Jackets Spring 2012 IEEE PES ICC Meeting Group A07D Selecting/Testing Jackets for Underground Cables March 27, 2012 Seattle, WA C.L. Flenniken 1 Outline
More informationEMPIRICAL AND MOLECULAR FORMULA
EMPIRICAL AND MOLECULAR FORMULA Percent Composition: law of constant composition states that any sample of a pure compound always consists of the same elements combined in the same proportions by mass
More informationPlastics. History of Plastics and Polymers
History of Plastics and Polymers Plastics Plastics are polymers. What is a polymer? The simplest definition of a polymer is something made of many units. Think of a polymer as a chain. Each link of the
More informationChapter 5. Name: Class: Date: Multiple Choice Identify the choice that best completes the statement or answers the question.
Class: Date: Chapter 5 Multiple Choice Identify the choice that best completes the statement or answers the question. 1. What is the pressure of the sample of gas trapped in the opentube mercury manometer
More informationTHE USE OF CRUDE OIL IN PLASTIC MAKING CONTRIBUTES TO GLOBAL WARMING
Département de Génie Energétique et Environnement INSA Lyon, France Department of Civil and Environmental Engineering Luleå University of Technology Luleå, Sweden THE USE OF CRUDE OIL IN PLASTIC MAKING
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationExploring Gas Laws. Chapter 12. Solutions for Practice Problems. Student Textbook page 477
Chapter 12 Exploring Gas Laws Solutions for Practice Problems Student Textbook page 477 1. Problem At 19 C and 100 kpa, 0.021 mol of oxygen gas, O 2(g), occupy a volume of 0.50 L. What is the molar volume
More informationFundamentals of Packaging Technology TABLE OF CONTENTS
Fundamentals of Packaging Technology TABLE OF CONTENTS Acknowledgements CHAPTER ONE  PERSPECTIVE ON PACKAGING What Is Packaging? Primitive Packaging From Rome to the Renaissance The Industrial Revolution
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationTECHNICAL DATA SHEET
POLYMERS Polyethylene (PE) Polypropylene (PP) Polyvinylchloride (PVC) Polystyrene (PS) Acrylonitrile Butadiene Styrene (ABS) Polymethyl Methacrylate (PMMA) Polyamide (PA) Polyacetal (POM) Polycarbonate
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More information75.5. Translate chemical symbols and the chemical formulas of common substances to show the component parts of the substances including:
75.5 Translate chemical symbols and the chemical formulas of common substances to show the component parts of the substances including: NaCl [salt], H 2 O [water], C 6 H 12 O 6 [simple sugar], O 2 [oxygen
More informationMole Notes.notebook. October 29, 2014
1 2 How do chemists count atoms/formula units/molecules? How do we go from the atomic scale to the scale of everyday measurements (macroscopic scale)? The gateway is the mole! But before we get to the
More informationIII. Synthesis A. Bulk polymerization 1. Initiator dissolved in monomer starts polymerization.
1 III. Synthesis A. Bulk polymerization 1. Initiator dissolved in monomer starts polymerization. 2. If polymer is soluble, then reaction mix increases viscosity. 3. If polymer is insoluble, viscosity remains
More informationSolution. Practice Exercise. Concept Exercise
Example Exercise 9.1 Atomic Mass and Avogadro s Number Refer to the atomic masses in the periodic table inside the front cover of this textbook. State the mass of Avogadro s number of atoms for each of
More informationPRACTICAL AND THEORETICAL CAPSULE
PRACTICAL AND THEORETICAL CAPSULE COMMON PLASTICS May 2008 WORKING DOCUMENT plastics_capsule_plastics_identification.doc 1 05/02/14 Objective: The objective of this capsule is to draw up a resume of the
More informationUnit X: Polymers Test 1.1
ame: Unit X: Polymers Test 1.1 Multiple hoice Questions 1 through 9 pertain to the reactions on the last two pages of this test. Where multiple answers exist only one need be reported. 1. Which process
More informationChapter 13. Conjugated Unsaturated Systems. Conjugation, Resonance and Dienes. Conjugation, Resonance and Dienes. What is the conjugation?
Chapter 13 Conjugation, Resonance and Dienes What is the conjugation? Conjugation occurs whenever p orbitals are located on three or more adjacent atoms. Conjugated Unsaturated Systems The four p orbitals
More informationBEYOND ELASTICITY. Subtopics. Plasticity Toughness Hardness Design problems
BEYOND ELASTICITY Subtopics 1 Plasticity Toughness Hardness Design problems PLASTICITY The stress is no longer proportional to strain 2 STRESSSTRAIN BEHAVIOR: PLASTICITY Tensile strength is the stress
More informationPractice questions for Ch. 3
Name: Class: Date: ID: A Practice questions for Ch. 3 1. A hypothetical element consists of two isotopes of masses 69.95 amu and 71.95 amu with abundances of 25.7% and 74.3%, respectively. What is the
More informationPS4.2 Explain how the process of covalent bonding provides chemical stability through the sharing of electrons.
PS4.1 Explain the role of bonding in achieving chemical stability. All of the noble gases are chemically stable A noble gas electron configuration (an outside energy level with 2 or 8 electrons) is chemically
More informationChemistry Stoichiometry. 45 points. Do not turn page until told to do so.
Chemistry 2010 Stoichiometry 45 points Do not turn page until told to do so. Stoichiometry Multiple Choice (Each worth 2 points) Identify the letter of the choice that best completes the statement or
More informationName Date Class CHEMICAL QUANTITIES. SECTION 10.1 THE MOLE: A MEASUREMENT OF MATTER (pages 287 296)
10 CHEMICAL QUANTITIES SECTION 10.1 THE MOLE: A MEASUREMENT OF MATTER (pages 287 296) This section defines the mole and explains how the mole is used to measure matter. It also teaches you how to calculate
More information2. If pressure is constant, the relationship between temperature and volume is a. direct b. Inverse
Name Unit 11 Review: Gas Laws and Intermolecular Forces Date Block 1. If temperature is constant, the relationship between pressure and volume is a. direct b. inverse 2. If pressure is constant, the relationship
More information
1/ 2. = 444 ms 1 PN RT. ρ = (πd 2 ) C rel ρ = m 3 s 1. = = mol L 1 s 1
TOPIC  THE COLLISIO THEORY Example of solved problems. For molecular oxygen at 5 o C, (a) calculate the collision frequency z and (b) the collision density Z at a pressure of atm. Given: d oxy. 0.36 nm.
More informationStoichiometry Dr. M. E. Bridge
Preliminary Chemistry Course Stoichiometry Dr. M. E. Bridge What is stoichiometry? The meaning of the word: The word stoichiometry comes from two Greek words: (meaning element ) and (meaning measure )
More informationMULTIPLE CHOICE. Choose the one alternative that best completes the statement or answers the question.
Chapter 10 MULTIPLE CHOICE. Choose the one alternative that best completes the statement or answers the question. 1) A gas at a pressure of 10.0 Pa exerts a force of N on an area of 5.5 m2. A) 1.8 B) 0.55
More informationCalculating Atoms, Ions, or Molecules Using Moles
TEKS REVIEW 8B Calculating Atoms, Ions, or Molecules Using Moles TEKS 8B READINESS Use the mole concept to calculate the number of atoms, ions, or molecules in a sample TEKS_TXT of material. Vocabulary
More informationof Lowenergy Plastics and Rubbers
6 Bonding of Lowenergy Plastics and Rubbers 6.1 Surface Wetting Silicone rubber, polytetrafluoroethylene (PTFE), Acetal and the polyolefin plastics (polypropylene, polyethylene) are always a challenge
More informationINTRODUCTORY CHEMISTRY Concepts and Critical Thinking
INTRODUCTORY CHEMISTRY Concepts and Critical Thinking Sixth Edition by Charles H. Corwin Chapter 9 The Mole Concept by Christopher Hamaker 2011 Pearson Education, Inc. Chapter 9 1 Avogadro s Number Avogadro
More informationMaster the elements. Unleash your potential.
Master the elements. Unleash your potential. Until now, traditional sterilization methods have restricted your potential. With superior compatibility across a wider range of materials, the REVOX method
More informationWebAssign Problem 1: When the temperature of a coin is raised by 75 C, the coin s. , find the coefficient of linear expansion.
Week 10 homework IMPORTANT NOTE ABOUT WEBASSIGN: In the WebAssign versions of these problems, various details have been changed, so that the answers will come out differently. The method to find the solution
More informationTutorial 6 GASES. PRESSURE: atmospheres or mm Hg; 1 atm = 760 mm Hg. STP: Standard Temperature and Pressure: 273 K and 1 atm (or 760 mm Hg)
T41 Tutorial 6 GASES Before working with gases some definitions are needed: PRESSURE: atmospheres or mm Hg; 1 atm = 760 mm Hg TEMPERATURE: Kelvin, K, which is o C + 273 STP: Standard Temperature and Pressure:
More informationResins for Optics. 1. LightCuring Resin 2. HeatCuring Resin. Introduction
Three Bond Technical News Issued July 1, 2004 63 Resins for Optics 1. LightCuring Resin 2. HeatCuring Resin Introduction As the word "optoelectronics is popular," the fields of electronics and optics
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationChapter 4 Polymer Structures. Chapter 4 Polymer Structures. Polymer Microstructure. Polymer Microstructure ISSUES TO ADDRESS...
hapter 4 Polymer Structures hapter 4 Polymer Structures ISSUES T ADDESS... What are the basic lassification? Monomers and chemical groups? Nomenclature? Polymerization methods? Molecular Weight and Degree
More informationIron is. Temperature is a(n) property of a substance. Select two that apply. Which of the following is a chemical change?
Posting ID: 419903 Course: CHE 105 2015 SU Instructor: Sarah Edwards Question #: 1 Iron is. A. a compound B. a heterogenous mixture C. a homogenous mixture D. an element Question #: 2 Temperature is a(n)
More informationNext, solid silicon is separated from other solid impurities by treatment with hydrogen chloride at 350 C to form gaseous trichlorosilane (SiCl 3 H):
University Chemistry Quiz 5 2014/12/25 1. (5%) What is the coordination number of each sphere in (a) a simple cubic cell, (b) a bodycentered cubic cell, and (c) a facecentered cubic cell? Assume the
More informationName Date Class CHEMICAL QUANTITIES. SECTION 10.1 THE MOLE: A MEASUREMENT OF MATTER (pages 287 296)
Name Date Class 10 CHEMICAL QUANTITIES SECTION 10.1 THE MOLE: A MEASUREMENT OF MATTER (pages 287 296) This section defines the mole and explains how the mole is used to measure matter. It also teaches
More informationPhysics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014
Physics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014 Part I: Shortanswer questions on basic principles. (5 points each) 1. Briefly describe the CZ method and the
More informationChapter 3: Stoichiometry
Chapter 3: Stoichiometry Goal is to understand and become proficient at working with: 1. Avogadro's Number, molar mass and converting between mass and moles (REVIEW). 2. empirical formulas from analysis.
More informationORGANIC AND BIOLOGICAL MOLECULES
APTER TWENTYTW RGANI AND BILGIAL MLEULES For Review 1. A hydrocarbon is a compound composed of only carbon and hydrogen. A saturated hydrocarbon has only carboncarbon single bonds in the molecule. An
More information"fluoromethane" Fluorine is able to pull electron density through the molecule, as it is being opposed by much less electronegative hydrogen atoms.
16 Examples: Polar? 1) POLAR BONDS? Yes. CF bonds should be polar. 2) SHAPE? The CF bonds are arranged in a tetrahedron. This makes the molecule symmetric and NONpolar, since the fluorines all pull against
More informationLota_2 Dæmi A3_ Sameindir og efni
Instructor Solutions Manual for Chemistry for Engineering Students, 2 nd Edition 81 Chapter 8 Lota_2 Dæmi A3_ Sameindir og efni 8.8 What is the difference between an amorphous solid and a crystalline
More information10 The Mole. Section 10.1 Measuring Matter
Name Date Class The Mole Section.1 Measuring Matter In your textbook, read about counting particles. In Column B, rank the quantities from Column A from smallest to largest. Column A Column B 0.5 mol 1.
More informationChapter 4 The Properties of Gases
Chapter 4 The Properties of Gases Significant Figure Convention At least one extra significant figure is displayed in all intermediate calculations. The final answer is expressed with the correct number
More information1 Material Properties of Plastics
j3 1 Material Properties of Plastics 1.1 Formation and Structure The basic structure of plastics (or polymers) is given by macromolecule chains, formulated from monomer units by chemical reactions. Typical
More informationChemical Engineering 160/260 Polymer Science and Engineering. Lecture 13: Polymerization Techniques  Dispersed Systems
Chemical Engineering 160/260 Polymer Science and Engineering Lecture 13: Polymerization Techniques  Dispersed Systems Objectives! To outline polymerization techniques and describe approaches to reducing
More informationRecall that ionic bonds form when the combining atoms give up or accept electrons. Another way that atoms can combine is by sharing electrons.
Molecular Compounds and Covalent Bonds Recall that ionic bonds form when the combining atoms give up or accept electrons. Another way that atoms can combine is by sharing electrons. Atoms that are held
More information